Dr. Dmitri Kopeliovich
Thermal barrier coatings (TBC) are ceramic layers deposited over metallic parts in order to provide their thermal insulation from the combustion gases.
Thermal barrier coatings allow to achieve higher efficiency of combustion engines (internal combustion engines and gas turbine engines) due to an increase of their operating temperature.
The method utilizes an electrical arc ionizing Argon flowing through it and converting into hot plasma at a temperature of about 15,000°F (8,300°C).
The ceramic material in powdered form is injected into the plasma jet where the ceramic grains melt and move in the stream of the hot gas towards the substrate surface.
When the molten particles impact the substrate surface they solidify in form of splats (flattened discs).
The resulting microstructure is composed of the grains and elongated pores stretched in the direction parallel to the substrate surface.
In EB-PVD technique an electron beam is directed to the target made of the ceramic material.
The electrons bombard the target and vaporize the material, molecules of which are accelerated towards the substrate surface.
The ceramic material deposits on the surface in form of parallel columns oriented perpendicualar to the substrate surface.
Because of its columnar structure the coatings produced by the method of electron beam physical vapor deposition have the thermal conductivity 30-40% higher than that of the coatings deposited by Air Plasma Spraying.
On the other hand the columnar structure is more tolerant to the stresses generated by thermal expansion of the coating.
Combustion chamber and blades of a gas turbine engine operate at high temperatures of about 2000°F (1093°C). The nickel base superalloys at such high temperatures are exposed to Creep and oxidation.
Thermal barrier coatings with the thickness allow to increase the service life of the turbine gas engine elements due to the protection of the metallic surface from oxidation and reduction of the substrate temperature by 212-500°F (100-260°C).
The directing blades, nozzle vanes and other elements of the combustion chambers are commonly coated by Air Plasma Spraying method.
The rotating blades are coated by Electron Beam Physical Vapor Deposition since the columnar grain structure of the coating is preferrable in the conditions of high thermallly induced stresses.
Maximum efficiency of a heat engine is:
ηmax = 1 - Tc/Th
Tc - temperature of the cold sink (cooling media), K;
Th - temperature of the hot source (combustion chamber), K.
According to the expression higher combustion temperature results in better theoretical efficiency of the engine.
In addition to this higher temperature causes the fuel burning to be more complete, which also increases the engine efficiency.
Higher temperature in the combustion chamber improves the engine efficiency.
The efficiency of conventional diesel engines is about 40%. 30% of the combustion gases energy is removed by the cooling system of the engine.
Thermal barrier coatings may increase the useful engine energy due to a reduction of the coolant energy.
The temperature of the combustion gases in a conventional diesel engine without thermal barrier coating is about 932°F (500°C). It may be increased up to 1472°F (800°C) by using a ceramic coatings over the diesel combustion chamber surface. The coating thickness is of order of 0.04” (1 mm).
Application of thermal barrier coatings in turbocharged diesel engines allows to increase the combustion gases temperature 2012°F (1100°C). At such high temperatures not only the engine efficiency is improved but also the content of the pollutants in the exhausting gases is reduced.
The main benefits of thermal barrier coatings in diesel engines: